Electronic Supporting Information Perylenediimide S1 Electronic Supporting Information Tunable...
Embed Size (px)
Transcript of Electronic Supporting Information Perylenediimide S1 Electronic Supporting Information Tunable...
Electronic Supporting Information
Tunable Low-Dimensional Self-Assembly of H-Shaped Bichromophoric
Perylenediimide Gemini in Solution
Yinjuan Huang,a Fei Yu,a Xun Cao,a Lina Nie,a Pengfei Zhang,b Fugui Xu,b Qiuyu Gong,a Xuejun Zhan,a Kexiang Zhao,a Yizhong Huang,a Yiyong Mai,*b Qichun Zhang*a
aSchool of Materials Science and Engineering, Nanyang Technological University, 639798, Singapore bSchool of Chemistry and Chemical Engineering, Shanghai Key Laboratory of Electrical Insulation and Thermal Ageing, Shanghai Jiao Tong University, 800 Dongchuan Road, Shanghai 200240, China
E-mail: email@example.com; firstname.lastname@example.org
Electronic Supplementary Material (ESI) for Nanoscale. This journal is © The Royal Society of Chemistry 2020
Materials. All the chemicals were purchased from Sigma-Aldrich, Merck, Alfa Aesar
and TCI suppliers, and were used as received unless otherwise described. Specifically,
perylene-3,4:9,10-tetracarboxylic dianhydride (97%), bromine (99.99 %), tin chloride
dihydrate (SnCl2·2H2O, 98%), potassium tert-butoxide (t-BuOK, 98%),
tris(dibenzylideneacetone)-dipalladium(0) (Pd2(dba)3, 97%), 1,3-bis(diphenylphosphino)
-propane (dppp, 97%) and potassium thioacetate (98%) were purchased from Sigma-
Aldrich. Dimethyl Formamide (DMF, HPLC), 1, 2-dichloroethane (DCE, 99.5 %), nitric
acid (fuming, 100%), dichloromethane (CH2Cl2, anhydrous, 99.8%), tetrahydrofuran
(THF, anhydrous, 99.9%), hexane (HPLC, 97%) and methanol (99.9%) were purchased
from Merck. 2-Octyldodecylamine (97%) was purchased from TCI, cerium (IV)
ammonium nitrate (98%) was purchased from Alfa Aesar. Anhydrous toluene was
distilled over Na/benzophenone under nitrogen after pre-dried with Na overnight. All the
self-assembly experiments were carried out using HPLC grade solvents. 200 mesh copper
grids (ZB-C4000) with ultra-thin carbon support film with thickness ≤ 3 nm were
purchased from Beijing Zhongxing Bairui Technology Co., Ltd. Silicon wafer (~ 0.25
cm2) was purchased from Shanghai Xinyang Semiconductor Materials Co., Ltd., which
was pretreated with O2 plasma for 20 min to make it more hydrophilic.
Characterization methods. Analytical thin layer chromatography (TLC) was carried out
on silica gel coated substrates bought from Merck. Hydrogen and carbon Nuclear
magnetic resonance (1H NMR and 13C NMR) spectra were recorded on a Bruker Advance
300 NMR spectrometer with tetramethylsilane as the internal reference and chloroform-d
(CDCl3) as solvents under ambient temperature. NMR data were collected via chemical
shift (ppm, CDCl3 resonance as the external standard), multiplicity and integration. All
the high-resolution mass spectra (HR-MS) were performed on a Waters Q-T of premier
mass spectrometer using acetone as solvent. Ultraviolet–Visible (UV–vis) absorption
spectra were performed on UV–vis–NIR Cary 5000 spectrophotometer.
Photoluminescence (PL) spectra were carried out via a Cary Eclipse Fluorescence
Spectrophotometer. Quartz cuvettes or plates were used for all the optical measurements.
Atomic force microscope (AFM) observations were completed on a scanning probe
microscope (AFM Asylum Research Cypher S, USA) operated via AC Mode Imaging
under atmosphere by using Arrow-NCR-50-Silicon SPM-Sensor cantilevers (side: Al-
coating, Coating: detector, force constant of 42 N m-1). AFM samples were prepared via
by drop-casting one drop (ca. 10 µL) of the assembly solution onto silicon wafer which was
placed on a piece of filter paper to remove most of the solvent, and then dried under vacuum
for 4 h at room temperature (RT). Scanning electron microscope (SEM) images were
collected on a JEOL/JSM-6340F under electric voltage of 5 kV. SEM samples were
prepared by drop-casting 5 drops (dropped one drop, dried, dropped, … repeated for 5
times, totally ca. 50 µL) of the assembly solution onto silicon wafer, and then dried under
vacuum for 4 h at room temperature (RT). Au spray was performed on the samples (30s)
to enhance the contrast before test. Transmission electron microscopy (TEM)
measurements were carried out on a JEM-2100 (JEOL Ltd., Japan) with accelerating
voltage of 200 kV. TEM samples were prepared by dropping the assembly solutions (ca.
10 µL) onto an ultrathin carbon-coated copper grids which was placed on a silicon wafer to
avoid spreading out of the solution, followed by drying under vacuum for 4 h at RT, and no
staining treatment was applied for TEM samples. The d-spacings in SAED patterns were
calibrated by gold nanoparticles standard. All the images were analyzed via the ImageJ
software developed by the US National Institute of Health. For the statistical analysis, ca.
200 assemblies were carefully traced manually to determine the dimension distributions
using ImageJ. Samples used for small and wide-angle X-ray scattering patterns (SAXS
and WAXS) tests were prepared by SD method, in which 10 mg PDI-NH-PDI was
dissolved in 1 mL toluene and then diffused into certain amount of hexane for 2 days.
Afterwards, dropping the self-assembled dispersion on a cleaned glass substrate, and
dried under vacuum before tests, which was fixed on the sample holder to perform test.
SAXS and WAXS analyses were recorded on a Xenocs Nanoinxider with Cu-Kα
microsource (40 mm, λ = 1.5 Å) at 30W under RT. Each collection was recorded using
medium resolution (MR) for 15 min. All the photos were taken by a Cannon EOS 700D
Synthesis of bromo perylene diimide (PDI-Br)1
DMF, reflux, overnight 2-Octyldodecylamine
bromine DCE, 80 oC, 1d
Scheme S1. Preparation of bromo perylene diimide (PDI-Br).
PDI was prepared according to the literature.2 Perylene-3,4:9,10-tetracarboxylic
dianhydride (5.1 mmol, 2.0 g) and 2-Octyldodecylamine (25.5 mmol, 5 eq., 7.6 g) were
suspended in 30 mL DMF in a 250 mL 1-neck flask equipped with a condenser. The
reaction mixture was degassed by argon bubbling, and then refluxed overnight under
nitrogen atmosphere. After reaction, the solution was cooled to RT, and 30 mL hydrogen
chloride (HCl) aqueous solution (1N) was added under stirring, the stirring was
maintained for 10 min. The resulted precipitate was collected by filtration and treated by
30 mL potassium hydroxide (KOH) aqueous solution (1M) to remove the excess HCl.
The precipitate was filtered again and washed with water until pH = 7 and dried under
vacuum at RT. Purification by silica gel column chromatography using eluent of
hexane/dichloromethane (DCM) (2/1, v/v) yielded PDI as as a dark red solid in 91%
yield. 1H NMR (300 MHz, CDCl3, Fig. S1): δ 8.69–8.51 (d, 4H), 8.51–8.32 (d, 4H), 4.25–4.00
(d, 4H), 2.15–1.82 (m, 2H), 1.48–1.18 (m, 64H), 0.98–0.75 (t, 12H). 13C NMR (300 MHz, CDCl3, Fig. S2): δ 163.51 (4C), 134.12 (4C), 131.15 (4C), 129.16
(2C), 126.03 (2C), 123.25 (4C), 122.84 (4C), 44.80 (2C), 36.75 (2C), 32.00 (6C), 31.85
(2C), 30.17 (4C), 29.74 (6C), 29.44 (4C), 26.62 (4C), 22.75 (6C), 14.18 (4C).
HR-MS (Fig. S3): m/z (%): 951.7011 (100) [M+H]+ (calcd. C64H91N2O4 = 951.6979).
Fig. S1. 1H NMR spectrum of PDI.
Fig. S2. 13C NMR spectrum of PDI.
Fig. S3. HR-MS spectrum of PDI.
Preparation of PDI-Br.1 A mixture of PDI (4 mmol, 2.9 g) and bromine (0.5mL, 10 mmol) in
60 mL of 1, 2-dichloroethane (DCE) was stirred at 80 °C in a closed round-bottom flask for 1 day.
Afterwards, the excess of bromine was removed by saturated sodium thiosulfate aqueous
solution via washing for 3 times. Then the organic phase was dried with anhydrous sodium
sulfate (Na2SO4) and then evaporated under vacuum. The crude product was purified via
silica gel column chromatography (eluent, hexane/DCM = 4/1, v/v), which afford bromo
perylene diimide as a red solid in 89% yield. 1H NMR (300 MHz, CDCl3, Fig. S4): δ 9.82–9.69 (d, 1H), δ 9.01–8.82 (s, 1H), δ 8.75–
8.59 (d, 3H), δ 8.58–8.36 (d, 2H), δ 4.25–4.01 (d, 4H), δ 2.20–1.75 (m, 2H), δ 1.51–1.12
(m, 64H), δ 0.98–0.75 (t, 12H). 13C NMR (300 MHz, CDCl3, Fig. S5): δ 163.65 (1C), 163.34 (1C), 163.24 (1C), 162.44
(1C), 139.07 (1C), 133.62 (1C), 133.25 (1C), 130.88 (4C), 130.44 (1C), 128.62 (1C),
128.43 (1C), 127.96 (1C), 127.76(1C), 126.71(1C), 123.53 (1C), 123.59 (1C), 123.39
(1C), 123.04 (1C), 122.83 (1C), 122.61 (1C), 120.96 (1C), 44.82 (2C), 36.70 (2C), 31.99
(6C), 31.81 (4C), 30.13 (2C), 29.41 (6C), 26.60 (2C), 22.75 (6C), 14.18 (4C).
HR-MS (Fig. S6): m/z (%): 1031.6075 (100) [M+H]+ (calcd. C64H90N2O481Br
Fig. S4. 1H NMR spectrum of PDI-Br.
Fig. S5. 13C NMR spectrum of PDI-Br.